Microstructure/Mechanical Property Relationships of...
Embed Size (px)
Transcript of Microstructure/Mechanical Property Relationships of...
Microstructure/Mechanical Property Relationships of Submerged Arc Welds in
HSLA 80 Steel
Submerged arc welds made at various energy inputs are evaluated in terms of microstructure and mechanical
properties, in both as-welded and stress-relieved conditions
BY N. J. SMITH, J. T. McGRATH, J. A. GIANETTO AND R. F. ORR
ABSTRACT. The relationship between microstructure and mechanical proper- ties was examined for weld metal and heat-affected zones of submerged arc welds deposited in HSLA 80 steel. The welds, deposited over an energy input range of 2-4 kj /mm (51-102 kj/in.) with two commercial consumable combina- tions, exceeded the targeted notch toughness properties in the as-welded condition. The superior toughness resulted from a high proportion of acicu- lar ferrite and low (O + S < 0.031) con- tent. The notch toughness of the coarse- grain heat-affected zone (CCHAZ) decreased with increasing energy input. The low toughness at the highest (4 kj/mm) energy input resulted from the increased proportion of CGHAZ taking part in the fracture and the formation of a coarse upper bainite microstructure. Stress relieving reduced the notch tough- ness of both the weld metal and heat-
As-Welded Properties Mechanical Properties Stress Relieved SA Welds in HSLA 80 Submerged Arc Welds 2-4 k j /mm Energy Input Coarse-Grain HAZ Notch Toughness Copper Precip. Steel Cu Precip. Hardening
N J. SMITH, I. T McGRATH, j . A. GIANETTO and R. F. ORR are with Metals Technology Laboratories (formerly Physical Metallurgy Research Laboratories), CANMET, Ottawa, Ont., Canada.
Paper presented at the 69th Annual AWS Meeting, held April 17-22, 1988, in New Orleans, La.
affected zone as a result of embrittle- ment caused by carbide precipitation and an increase in yield strength resulting from copper precipitation.
Current interest in the fabrication of naval surface ships and submarines has prompted renewed studies on sub- merged arc welding of conventional high-strength quenched-and-tempered (Q&T) steels, particularly HY 80 (Ref. 1) and HY 100 (Ref. 2). Recently, several papers have been published on the development of copper-precipitation- strengthened steels that have potentially the same (or better) strength and tough- ness properties, with improved weldabili- ty compared to the conventional Q&T steels (Refs. 3-5). One of these steels, designated HSLA 80, is a modified version of ASTM A710 Grade A Class 3, and is currently being specified for the con- struction of U.S. Navy ships (Ref. 6).
HSLA 80 steel differs from the conven- tional higher-carbon quenched-and-tem- pered HY steels in that the strength is obtained through copper precipitation hardening. The steel has lower carbon and alloy levels, and therefore does not transform to the hard martensitic struc- ture associated with the HY steels. This leads to improved weldability and essen- tially eliminates the need for preheating at ambient temperatures above 0°C (32°F). However, only limited published research exists on the evaluation of weldability and mechanical properties of weldments in ASTM A710 (Refs. 7, 8) and HSLA 80
(Refs. 9-11). The recent work of Jesse- man and Schmid (Ref. 7) focused on the evaluation of copper-containing steels (ASTM A710 Grade A and ASTM A736), with the aim of determining the effects of base plate heat treatment class, welding energy input, and plate thickness-heat flow conditions on the HAZ toughness and hardness. They also reported weld metal properties for several welding con- sumable combinations for both the as- welded and PWHT conditions. However, in order to establish the suitability of the HSLA 80 steel for critical applications and to provide guidance with regard to weld- ing procedure development, there is a need for further research to obtain more quantitative results on structure/property relationships of weld metals and heat- affected zones. The objective of the present study was to perform a quantita- tive analysis of the microstructure/ mechanical property relationships of sub- merged arc welds deposited in low- carbon, copper-precipitation-strength- ened HSLA 80 steel.
Base Material and Welding Procedure
Microstructure and mechanical prop- erty studies were performed on experi- mental submerged arc welds deposited in 25.4-mm (1-in.) thick HSLA 80 steel, the composition of which is listed in Table 1. The mechanical property requirements presented in Table 2 were established from current military standards con- cerned with the qualification of sub-
Table 1—Chemical Composition of HSLA 80 High-Strength Steel
Element, wt-% C Mn Si S P Ni Cr Mo Cu V Nb
0.060 0.50 0.27 0.004 0.007 0.92 0.66 0.25 1.02 0.005 0.044
112-s | MARCH 1989
(a) 2 k J/mm
(b) 3 kJ/mm
Typical Charpy Location
Fig. 1—joint design preparation, pass sequence and Charpy specimen location for the submerged-arc welds
Fig. 2 — Schematic diagram showing position of HAZ Charpy specimen, notched through thickness, 1 mm from the fusion line
merged arc welding consumables for HY 80/100 steels (Ref. 12).
Two series of submerged arc welds (Series A and Series B) were made using electrode/flux combinations approved for welding HY 80 at energy inputs less than or equal to 4 k j /mm (102 kj/in.). The two electrodes used were both 100S-1 (AWS EM2) classification, and the two fluxes were highly basic. The consuma- bles, weld identifications, and welding parameters are listed in Table 3. The ranges of energy inputs employed were in accordance with the limits specified for HY 80 steels in the current military stan- dard for HY 80/100 submarine construc- tion (Ref. 13). Single-V joint design prepa- rations were used with a 60-deg included angle and a 6- to 8-mrm (0.24- to 0.31-in.) root face, to accommodate increasing energy input. Figure 1 shows the joint design preparation, pass sequence and Charpy test specimen location. The welds were air carbon arc back gouged on the second side prior to deposition of the final passes. All welding was done parallel to the plate rolling direction.
To evaluate the microstructure and mechanical properties of both as-welded and stress-relieved conditions, one half of each weld from Series A was subjected to a PWHT for 1 h at 600°C (1112°F) for stress relieving (SR). All the welds were inspected by x-ray radiography prior to machining mechanical test specimens.
Mechanical Testing and Metallography
The tensile properties were deter- mined from all-weld-metal specimens for the Series A and B as-welded condition and the Series A stress-relieved condition. Charpy impact transition curves were generated for each test condition, includ- ing both weld metal and the CGHAZ
regions. The specimens were notched through-thickness at the weld centerline and the CGHAZ 1 mm (0.04 in.) from the fusion line on the back gouged side of each weldment, as shown in Figs. 1A and 2, respectively.
The microstructures of the weld metal and the CGHAZ were identified and char- acterized using optical and scanning elec- tron microscopy (SEM) for both the as- welded (AW) and the stress-relieved (SR) conditions. The specimens were pre- pared by standard metallographic tech- niques and subsequently etched in 2% nital to reveal the overall structure and in 4% picral for details of secondary micro-
constituents, M-A and/or carbides. Point counting was performed on the last as- deposited weld bead to determine the percentage of acicular ferrite (AF), grain boundary ferrite (GF), ferrite with second phase (FS) (aligned FS(A) and nonaligned FS(N)), and polygonal ferrite (PF) in accor- dance with current IIW recommenda- tions (Ref. 14). Transmission electron microscopy was used to study copper precipitation in selected samples, using a two-stage carbon extraction replica tech- nique. Energy dispersive x-ray analysis was used to determine the precipitate compositions.
Fractured surfaces of selected Charpy
Table 2—Mechanical Property Requirements for HSLA Submerged Arc Weld Metals
Yield strength Reduction in area
Elongation Charpy impact energy
565 MPa min 50% min 20% min
81 J at -18°C 47 J at -50°C
Table 3—Submerged Arc Welding Consumables and Parameters
SA20 SA30 SA30
SA21 SA31 SA41
Energy Input, k j /mm
2 3 4
2 3 4
Electrode A 100S1 (EM2)
Basic flux B.l. = 3.0*
Electrode B 100S1 (EM2)
Basic flux B.l. = 2.7*
450 500 570
450 500 570
Wire Feed Speed,
55.0 61.2 76.2
55.0 61.2 76.2
Travel Speed, mm/s
7.8 5.9 5.1
7.8 5.9 5.1
Note: a) voltage setting — 35 V; b) electrode extension — 32 mm; c) preheat temperature — 93°C; d) interpass temperature - 149°C; e) electrode diameter —2.4 mm. *Basicity index was provided by manufacturer.
WELDING RESEARCH SUPPLEMENT 1113-s
Table 4—Chemical Composition of Submerged Arc Welds
Weld Series No.
SA20 A SA30
SA21 B SA31
Note: For all weld metals,
Electrode A 100S-1
Electrode B 100S-1
0.06 0.05 0.06
0.05 0.05 0.05
Nb = 0.020